Presentation on theme: "MarineMend Repair Kit Procedure"— Presentation transcript:
1MarineMend Repair Kit Procedure For MarineLine Coated Tanks
2PurposeThe purpose of this procedure is to clearly explain what must be done in order to repair a tank for service. The repair procedure should be used when the coating has been misapplied, damaged, or contains holidays (pinholes).
3SafetyObserve ALL safety requirements during this procedure, including wearing all safety equipment
7Pre-Surface Preparation Pre-Surface Preparation includes a detergent wash and chemical cleaning of all surfaces to be repaired.All surfaces must then be dried
8Surface PreparationIf the damaged areas are small and independent (separate) from each other, the small damaged areas may be hand sanded with a medium grit aluminum oxide sandpaper. Sand the topcoat (grey) of the MarineLine coating, and any rust spots must be removed.
10Surface PreparationFor areas that are larger, a disk sander with a medium grit aluminum oxide disk should be used. Remove topcoat (grey) of the MarineLine coating, and any rust spots down to a near white metal.Note: All areas sanded down to a near white metal, must have an area of 25 mm around it’s periphery. MarineLine coating topcoat (grey) removed to a feathered edge.
18Coating The Repair Spots When all preparation work is completed mix thoroughly the MarineMend Repair Kit. Part A (Resin) with Part B (Catalyst).Note: The pot life of the MarineMend Repair Kit is 15 minutes 20CMake sure all surface preparation is completely finished before mixing the kit.
25Coating The Repair Spots Apply one coat of the MarineMend Repair Kit to the prepared surface area. The final average dry film thickness (DFT) should measure 300 microns. At NO TIME should the average DFT exceed 350 microns.
29Coating The Repair Spots Allow to dry for 6 – 8 hours with good ventilation
30No Heat Curing Required No heat curing is required when using the MarineMend Repair Kit
31No Heat Curing Required Chemical resistance for carrying clean products will develop in 7 days at 24 C.
32No Heat Curing Required Full chemical resistance per the chemical resistance guide will develop as follows:30 days at 24 C40 days at 20 C60 days at 15 C90 days at 10 CDo not allow temperature to drop below 10 C
33SafetyObserve ALL safety requirements during this procedure, including wearing all safety equipment